Highly photoluminescent two-dimensional imine-based ... paper/ آ Highly photoluminescent
Embed Size (px)
Transcript of Highly photoluminescent two-dimensional imine-based ... paper/ آ Highly photoluminescent
This journal is©The Royal Society of Chemistry 2018 Chem. Commun., 2018, 54, 2349--2352 | 2349
Cite this:Chem. Commun., 2018, 54, 2349
Highly photoluminescent two-dimensional imine- based covalent organic frameworks for chemical sensing†
Qiang Gao, ‡ab Xing Li, ‡b Guo-Hong Ning, b Kai Leng,b Bingbing Tian, ab
Cuibo Liu,ab Wei Tang,c Hai-Sen Xub and Kian Ping Loh *ab
The strong p–p interactions in the stacking layers of two-dimensional
covalent organic frameworks (2D-COFs), together with rotationally
labile imine linkages, make most of the solid state imine-linked COFs
non-fluorescent due to fluorescence quenching processes. Here, we
report the successful synthesis of highly photoluminescent imine-based
2D-COFs by integrating a non-planar building unit with a pyrene-based
unit and transforming the COF into spherical, sub-micron particles. High
photoluminescence quantum yields (PLQY) were achieved with COF
sub-micron particles dispersed in organic solvents. The as-prepared
COF sub-micron particles can be used as a chemical sensor for the
detection of explosive chemicals, with high sensitivity and selectivity
(up to ppm level).
Covalent organic frameworks (COFs) are an emerging class of ordered conjugated organic polymer materials constructed through the covalent linkages of organic building blocks via reversible bond formation chemistry.1 Enjoying the advantages of low densities, high surface areas and thermal stabilities, COFs show broad applications in gas storage,2 heterogeneous catalysis,3 chemical sensors,4 drug delivery,5 energy conversion and storage6 etc. In general, 2D-COFs are assembled via p–p stacking interactions, thus the aggregation- caused quenching (ACQ) effect results in non- or less-emissive 2D-COFs. Highly emissive 2D-COFs based on fluorescent pyrene and aggregation-induced emission (AIE) building units had been reported using the boronate ester linkage4b and azine-linkage.4a
However most of the imine-linked 2D-COFs reported previously were non- or weakly fluorescent.7 To prevent fluorescence quenching
by strong p–p stacking interactions, Wang et al. demonstrated a pyrene-based fluorescent 3D imine COF (3D-Py-COF).4g Apart from the 3D bonding framework, the synthesis of highly photolumines- cent 2D-COFs linked by imine bonds remains a challenge.
To achieve highly emissive 2D-COFs, Jiang et al. designed a boronate ester based 2D-COF consisting of an aggregation- induced emission (AIE) moiety (TPE-Ph COF).4b Imine COFs, with higher stability and easier chemical conversion,8 are more suited than boronate ester-linked COFs for applications in catalysis, gas adsorption and chemical sensors. Although strong photolumines- cence can be seen in boronate ester-linked COFs, there has been no photoluminescent tetraphenylethene (TPE)-based imine COFs reported thus far. Herein, we develop a general strategy for constructing a highly luminescent imine-based 2D-COF based on the integration of a non-planar TPE building unit with a pyrene unit (Fig. 1), and engineering the morphology of the COF into spherical, sub-micron sized particles. High photo- luminescent quantum yield (up to 21.1%) is achieved from COF nanoparticles that are dispersed in organic solvents. Furthermore, our pyrene-TPE-based imine 2D-COF (Py-TPE-COF) nanoparticles can be used to sense explosive chemicals with high sensitivity and selectivity (up to ppm level).
To construct our Py-TPE-COF, 1,3,6,8-tetrakis(4-aminophenyl)- pyrene (1) is chosen as the amine unit because of the fluores- cence properties of the pyrene motif. Due to the topology and assembly rules of building blocks, the non-planar 1,1,2,2- tetrakis(4-formylphenyl)ethane (TPE-4CHO, 2), with the function of AIE, is selected as the aldehyde unit. To our delight, a highly crystalline Py-TPE-COF has been successfully synthesized via [4+4] imine condensation under solvothermal conditions (ESI†). To confirm the formation of the imine bond linkage in the Py-TPE-COF, Fourier transform infrared spectroscopy (FT-IR) and solid state 13C CP-MAS NMR characterization were performed. The FT-IR spectrum of the Py-TPE-COF shows the stretching vibration band of the imine bond (–CQN–) at 1622 cm�1, while model compounds Py-M and TPE-M (Fig. S1, ESI†) also display the similar CQN vibration bands at 1625 cm�1 and 1624 cm�1, respectively (Fig. S10, ESI†). Solid state 13C CP-MAS NMR
a SZU-NUS Collaborative Innovation Center for Optoelectronic Science &
Technology, Key Laboratory of Optoelectronic Devices and Systems of Ministry of
Education and Guangdong Province, College of Optoelectronic Engineering,
Shenzhen University, Shenzhen 518060, China b Department of Chemistry, Centre for Advanced 2D Materials (CA2DM), National
University of Singapore, 3 Science Drive 3, Singapore 117543, Singapore c Institute of Materials Research and Engineering, A*STAR, 2 Fusionopolis Way,
Innovis, Singapore 138634, Singapore. E-mail: email@example.com
† Electronic supplementary information (ESI) available. See DOI: 10.1039/ c7cc09866a ‡ These authors contributed equally to this work.
Received 26th December 2017, Accepted 5th February 2018
l U ni
View Article Online View Journal | View Issue
http://orcid.org/0000-0002-8783-3245 http://orcid.org/0000-0002-5470-1043 http://orcid.org/0000-0002-5640-9062 http://orcid.org/0000-0003-1508-6217 http://orcid.org/0000-0002-1491-743X http://crossmark.crossref.org/dialog/?doi=10.1039/c7cc09866a&domain=pdf&date_stamp=2018-02-12 http://rsc.li/chemcomm http://dx.doi.org/10.1039/c7cc09866a http://pubs.rsc.org/en/journals/journal/CC http://pubs.rsc.org/en/journals/journal/CC?issueid=CC054019
2350 | Chem. Commun., 2018, 54, 2349--2352 This journal is©The Royal Society of Chemistry 2018
spectroscopy of the Py-TPE-COF reveals a characteristic reso- nance signal at 157.4 ppm, further confirming the presence of CQN imine bonds (Fig. S8, ESI†). In addition, thermal gravimetric analysis (TGA) shows that the Py-TPE-COF is thermally stable under a nitrogen atmosphere (up to 400 1C, Fig. S9, ESI†). Elemental analysis of the Py-TPE-COF reveals that the contents of carbon, hydrogen, and nitrogen of the COF are 87.24%, 4.30%, and 5.81%, respectively, which are close to the theoretically calculated values (89.53% for C, 4.51% for H, and 5.97% for N).
The crystallinity of the Py-TPE-COF is determined by powder X-ray diffraction (PXRD) analyses using Cu Ka radiation (Fig. 2 and Fig. S3, ESI†). The observed PXRD patterns of the Py-TPE- COF exhibit PXRD peaks at 5.851, 8.561, 11.671, 13.421, 17.401 and 19.531, which could be assigned to the (220), (400), (440), (260), (660), and (001) planes, respectively (Fig. 2a). To further determine the crystal structure of the Py-TPE-COF, theoretical simulations are carried out using Materials Studio (version 2016, ESI†). Unit cell parameters of a = 42.63 Å, b = 43.72 Å, c = 4.57 Å, a = g = 901, and b = 78.81 with the C2/m space group are obtained through geometry and energy minimization (Table S1 and Fig. S26–S29, ESI†). The simulated PXRD patterns of the eclipsed structure show very good agreement with the experimental PXRD patterns, either in peak positions or in relative intensities (Fig. 2b and d). Furthermore, the Pawley- refined PXRD profiles match the experimental PXRD patterns very well with Rwp of 2.73% and Rp of 2.09% (Fig. 2a). However, the calculated PXRD pattern for the staggered structure does not agree with the experimental PXRD patterns (Fig. 2c and e), thus we exclude the possibility of the staggered stacking mode in the Py-TPE-COF.
The permanent porosity of the Py-TPE-COF is investigated by nitrogen sorption measurements at 77 K, after being activated by degassing the COF sample at 120 1C for 8 h (Fig. 3a). The Brunauer–Emmett–Teller (BET) surface area and pore volume
are calculated to be 987 m2 g�1 and 0.77 cm3 g�1 (P/P0 = 0.983), respectively. The pore-size distribution is calculated based on nonlocal density functional theory (NLDFT), resulting in a micropore size centered at 1.1 nm (Fig. 3a, inset), which shows good agreement with the pore size predicted from the crystal structure of the Py-TPE-COF (1.2 nm). The morphology of the Py-TPE-COF is revealed by scanning electron microscopy (SEM) to be spherical (Fig. 3b and Fig. S24, ESI†). Transmission electron microscopy (TEM) images of the Py-TPE-COF also reveal that the COF crystallizes in the form of sphere-like nanoparticles with domain sizes of 300–500 nm (Fig. 3c and Fig. S25, ESI†), this observation is consistent with the nano- particle size shown in the SEM characterization.
To our delight, Py-TPE-COF nanoparticles, which are dis- persed well in tetrahydrofuran (THF), display a bright blue photoluminescence (PL) which is visible with the naked eye when excited by 365 nm ultraviolet lamps (Fig. 4a, inset c; and Fig. S14, ESI†). This directly confirms the highly fluorescence emission of Py-TPE-COF nanoparticles dispersed in organic solvents. UV-Vis spectra show that the model compounds (TPE-M and Py-M) exhibit absorption peaks at 363 nm and 401 nm, respectively, whereas the Py-TPE-COF exhibits an absorption peak centered at 401 nm (Fig. S18, ESI†). Under 365 nm